175,000 Device-Hours Operation of AlGaN/GaN ... 175,000 Device-Hours Operation of AlGaN/GaN HEMTs on
Embed Size (px)
Transcript of 175,000 Device-Hours Operation of AlGaN/GaN ... 175,000 Device-Hours Operation of AlGaN/GaN HEMTs on
Abstract—Hundred and seventy-five thousand device-hours of
operating life at channel temperatures above 200°C is demonstrated on AlGaN/GaN HEMTs fabricated using GaN-on- diamond technology for the first time. No catastrophic failures and no drain-current drift larger than 10% from turning the devices on were recorded throughout this two-year DC test.
Index Terms—diamond, gallium nitride, semiconductor device reliability, transistors
HE introduction of new semiconductor-device technologies carries a burden of proof that not only their
performance and price can offer advantages over exiting technologies, but that the devices exhibit reliability sufficient for commercial deployment. The interest in AlGaN/GaN high- electron mobility transistors (HEMT) as potential work-horse of high-power RF and power-management applications has spurred great interest in their reliability , , . AlGaN/GaN HEMTs are traditionally fabricated on sapphire, silicon carbide, or silicon. Growing GaN on these heterogeneous substrates necessitates the incorporation of nucleation layers between the substrate and the high-quality GaN epilayers. This approach carries multiple disadvantages from thermal management point of view: some substrates have poor thermal conductivity, while the nucleation layers exhibit significant thermal boundary resistance in addition to their low bulk thermal conductivity (< 25 W/mK) resulting from the high dislocation density and use of AlGaN ternary alloys. The recent attempts to minimize or alleviate some of these problems comprise attempts to integrate GaN with diamond , , , , , . The approach of Group4 Labs, in which GaN epilayers are atomically attached to chemical- vapor deposited (CVD) diamond wafers has up to now exhibited great progress by demonstrating 100-mm GaN-on- diamond wafers , devices with fT ~ 85 GHz , and X- band amplifiers . GaN-on-diamond technology not only replaces the original, growth substrate with diamond but it
Manuscript received March 11, 2012. This work was supported in part by
the US NAVY SBIR Phase II Contract number N0002409C4164 and AFRL Contract number FA865009C5404.
Dubravko I. Babić, Quentin Diduck, Chandra S. Khandavalli, Daniel Francis, Firooz Faili, Felix Ejeckam are with Group4 Labs, Inc., Fremont, California, CA 94539. (e-mail: firstname.lastname@example.org).
also allows the removal of the poorly thermally conductive nucleation layers prior to attaching the epilayers to diamond.
The reliability of devices built by processes in which epilayers are transferred from the growth substrate to another substrate, such as, epitaxial liftoff, wafer bonding, and atomic attachment, understandingly undergo special scrutiny of the components community because mechanical handling of thin epilayers is more likely to introduce damage and stresses to the semiconductor epilayers and/or the device than traditional semiconductor fabrication in which the epilayers stay attached to the as-grown substrate. In addition, atomic attachment relies on several high-temperature process steps. Therefore, the central question posed by many interested users of this technology is whether GaN-on-diamond devices will last. This paper contains the first report of high-temperature operating life (HTOL) experiments on GaN-on-diamond high- electron mobility transistors.
The primary objective of this experiment was to check whether these devices would “last through the weekend”. The result was surprising, as up to date over 175,000 device-hours have been collected on devices that operate with channel temperatures above 200°C, IDS ~ 60 mA/mm, and VDS up to 48 V. We describe the device design, the experimental setup, and the results of the first two-year operating life test on GaN- on-diamond HEMTs.
II. DEVICE STRUCTURES AND LIFE-TEST DETAILS AlGaN/GaN high-electron mobility transistors (HEMT)
were fabricated on GaN-on-diamond wafers with layer structure shown in Figure 1. Gallium-nitride on silicon wafers were purchased with standard epilayer design from Nitronex, Inc. and the GaN epilayers were transferred onto diamond using Group4 Labs’ atomic attachment process . The wafers used in this work were of the first generation of GaN- on-diamond devices in which the nucleation layers (shown in Figure 1) are still present. The wafers were processed at MicroGaN in Ulm, Germany. Free-standing GaN-on-diamond wafer diameter was 24 mm and the wafers were attached to 100-mm silicon wafers for processing.
The layout contained a variety of two gate HEMTs with no air-bridges. The gate metallization was Ni/Au, while silicon nitride was used for passivation. Device physical dimensions
175,000 Device-Hours Operation of AlGaN/GaN HEMTs on Diamond
at 200°C Channel Temperature Dubravko I. Babić, Senior Member, Quentin Diduck, Member, Chandra S. Khandavalli,
Daniel Francis, Firooz N. Faili, Member, and Felix Ejeckam
MIPRO 2013, May 20-24, 2013, Opatija, Croatia
were W = 2 × 400 μm, LG = 1.2 and 2 μm, LGD = 3, 4, and 5 μm. We could not resolve the effect of these dimensional variations on the performance nor the reliability, hence, in the test we treated the devices as being identical. The wafers were diced using Q-switched Nd:YAG laser . The final chip size was 1.5 x 1.5 mm and it contained two HEMTs per chip. The chips were packaged into Stratedge 580286 packages using silver epoxy. The reason for silver epoxy was that solder could not wet the rough diamond back-surface; the back of the diamond wafer on these experimental devices was not coated with metal. The package lid was omitted.
Figure 1 – GaN-on-diamond HEMT epilayer structure
Figure 2 – Electrical wiring: (a) common source resistor, and (b) separate source resistors. The two transistors in the dashed-line box represent the two halves of a two-source HEMT on a chip. The devices were self-biased according to the electrical
scheme shown in Figure 2 which allows biasing and real time measurement of IDS at constant VDS with a single wire per device (also: single power supply and one meter per device). The transistor was stabilized using short bondwires and negative feedback (RS) chip resistors inside the package. The two electrical circuit diagrams shown in Figure 2 are equivalent provided that the two sides of the two-gate transistors have identical DC characteristics. We first used diagram from Figure 2(a) with RS = 25 Ω (Table 1, Groups 1- 3), but subsequently realized that the circuit layout with two separate sources, common to microwave transistors, enables one to use separate source DC operating point stabilizing resistors RS as shown in Figure 2(b) and photo in Figure 3. Using separate source resistors in each of the two sources
reduces the difference between the drain currents in the two transistor halves when the transconductance differs on the two transistor halves. We estimated the reduction in the difference between the drain currents of the two halves for the transistors under test. For typical values of IDSS ~ 70 mA and VTH ~ �1.3 V at operating temperature, using separate 10 Ω (2RS) resistor in each source, as in case (b), rather than connecting both sources to ground via a single 5 Ω (RS) resistor, as in case (a), results in about 20% reduction in the sensitivity of the difference between the drain currents to device parameters. This separate biasing was implemented on Group 4 devices in Table 1.
Figure 3 – Photograph of the wirebonding of a single two- source HEMT with two source resistors according to schematic shown in Figure 2.
Figure 4 – The effect of transconductance or threshold voltage drift on measured drain current
The test system contained a number of 24V and 48V DC
power supplies; one power supply and a dedicated analog panel ammeter per device. Analog meters offer practically infinite failure-free operation (no batteries) and no common electrical power supply lines. (Note that with the return path (ground) being common to all the devices in Figure 2, both
ammeter terminals have to be floating to make independent measurements of the drain current. The drain current data acquisition was done with no interruption to the device operation.
Figure 5 – Typical room-temperature DC characteristics (IDS vs. VDS) for devices under test connected using circuit diagram shown in Figure 12. The reduction in IDS with voltage is due to self-heating and it is more pronounced for devices biased at 48V.
III. RESULTS The operating characteristics of the HEMTs can drift in
many ways during a life test. Using the circuit layout shown in Figure 2, we are primarily sensitive to the changes in IDSS and VTH. We do not monitor gate leakage. Figure 4 illustrates how drift in VTH and/or IDSS affects the IDS readout. Clearly, if IDSS reduces with time, the readout IDS will follow proportionally. If the threshold voltage VTH changes, the transfer characteristics will shift and IDSS will change again producing a change in the readout IDS. In Figure 4, this is illustrated with IDS1 changing to IDS2 as VTH1 changes to VTH2. The goal is to note any gross change in device characteristics and observe any catastrophic failures. Inasmuch as there was no prior knowledge of what the outcome of this test would be, the devices were planned for a range of different stress levels: The two different bias voltages VDS, two different starting drain current levels IDS, and two di